INDUXTRIAL AND ENGINEERING CHEMISTRY
Vol. 20. No. 5
Effect of Heat on Raw Rubber' C. R. Park, C. M. Carson, and L. B. Sebrell THEGOODYEAR TIRE& RUBBER Co., AKRON,OHIO
Effect on Plasticity
It may be seen that the increase in plasticity occurs N THE report of the Physical Testing Committee2 and whether or not the heating is done in the presence of steam in a communication by one of the writers,3 it is pointed and that the breakdown corresponds roughly to about out that when rubber is milled upon rolls of relatively four or five passes through a fairly tight mill. high temperature a less plastic milled product is obtained Effect on Chemical Characteristics than when the rolls are cold. The high temperature of the mill results in a temporary softening, which makes the rubber At this point in the investigation it was discovered that a less susceptible to the mechanical action of the rolls. The pronounced increase in rate of cure of the rubber was brought result of this behavior is that any permanent effect of heat about by the heating. This effect was noted in two mixes; per se during milling on hot rolls is completely masked by in one the time of cure was reduced from 3 hours at 141 O C. the enormously greater effect of the mechanical action. to less than 21/2 hours a t 141' C., and in the other: from 45 It has been stated by Worthington and Hyde4 that when minutes at 125' C. to less than 30 minutes at 125' C. The raw rubber is heated in steam a t 10 to 60 pounds pressure heated rubber was always foul in odor and when fresh from the for 7 hours the plasticity is autoclave sometimes smelled increased. It is of interest decidedly of amines and A study has been made of the effect of heat upon to know whether the plasammonia. It was thought ticizing effect so obtained is crude rubber. Heating in steam for 24 hours at 158' C. t h a t protein hydrolyplastifies the rubber to about the same extent as about of the order of magnitude of sis was responsible for the five passes through a tight mill. The chemical charthat obtained by milling and odor and the increased rate acteristics are changed in such a way as to indicate that whether the heating during of cure, and so a more coma portion of the protein materials and fatty acid esters milling is a small contributprehensive series of experihas been hydrolyzed. The rate of cure is increased in ing factor to the permanent ments was carried out to get the case of most crudes for mercaptobenzothiazole and plasticity. a more accurate idea of the pure-gum mixes, but is less affected in the case changes taking place i n the Several samples of rubber of hexamethylenetetramine, diphenylguanidine, and rubber and the effect of these were heated in a small autoethylidene aniline. The stress-strain curve is affected c h a n g e s u p o n cure with clave with water, care being by the heating in such a way as to make it more convex various accelerators. taken to sweep out the air toward the strain axis. The apparatus consisted with steam. The heating A study has been made of the chemical constituents was continued for periods of of a steel autoclave 13 inches (33 cm.) deep by 8 inches of the heated rubber which have been responsible for one day and the samples changes in curing characteristics. It is believed that (20 cm.) in diameter capawere then air-dried to transthe amines, nitrogen bases, and alkaloids are the ble of holding 8 to 10 kg. of parency. I n each case an principal active material responsible for the peculiaricrude rubber. It was proincrease in plasticity was obvided with a bolted-on lid, tained over t h e o r i g i n a l ties of heated rubber. lead gasket, and blow-off sample. valve. About 1 liter of Table I gives comDarisons of the becavior of t h e rubber with various heat treatments water was added. The autoclave was placed in a horizontal and milling. A uniform sample of smoked sheet which had pot heater and heated for 10 minutes a t 158' C. in steam. been blended in a large batch on an 80-inch (203-cm.) mill The heater was then opened and the blow-off valve of the autoclave opened for 5 minutes to allow steam to drive out was used. the air present when the autoclave was charged. The blowTable I-Effect of Various Heat Treatments and Milling on Plasticity off valve was then shut, the heater closed, and the rubber PASSES THROUGH METHOD OF HEAT COOL MILLAT heated for 24 hours a t 158' C. TREATMENT.' 1 MM. GAGE PLASTICITYRECOVERY In Table I1 is presented the effect of this heat and steam Min. Min. treatment on several different types of rubber. The first 4.75 0.63 Control N o treatment effect of heating noted is the increase in the acetone extract, 0.26 3.69 Steam 3.81 0.19 Dry (in press) which may be due to partial depolymerization of the rubber 4.38 0.42 itself, thus rendering it acetone-soluble. Another source of 4.27 0.33 0.25 4.15 increased acetone extract may be the protein hydrolysis 0.19 3.96 0.16 3.69 products. The second effect is the increase in acid number, 0.11 3.64 as determined on the acetone extract by the method of a At 158O C. and 5 kg. per sq. cm. (70 Ibs.) pressure for 24 hours. Whitby and Winn.5 This is probably caused by the effect Plasticity is the thickness in millimeters of a 2-cc. pellet of heat, pressure, and steam in hydrolyzing the fatty acid after 3 minutes at 70" C. under a 5-kg. load in the Williams esters (glycerol salts of the fatty acidsB), and also by the plastometer. Recovery is the increase in thickness when hydrolysis of the rubber protein and formation of free amino acids. The third effect is the increase in the acetone-soluble measured immediately after removal from the press. nitrogen at the expense of the acetone-insoluble, and may 1 Presented before the Division of Rubber Chemistry at the 74th be caused, as previously stated, by an increased solubility in Meeting of the American Chemical Society, Detroit, Mich., September 5 to
10,1927. * IND.END.CSBM.,1'7, 635 (1925). 8 Park, Rubber Age (London), 6, 630 (1925). 4 U. S. Patent 1,360,486(1920).
J . SOC.Chcm. I n d . , 42,336T (1923). Lewkowitz, "Chemical Examination of Oils, Fats, and Waxes," 5th ed., Vol. I , p. 77. 5 6
INDUSTRIAL A N D ENGINEERING CHEMISTRY
acetone of the protein hydrolysis products Over the original be noted that the total rubber proteins. ~t should nitrogen after heating is in all cases less than before heating, showing that the ammoniacal odor on opening the autoclave was really due to volatile nitrogenous substances. Effect upon C u r e
A more thorough investigation of the effect of heating rubber was next undertaken. Several different types of rubber in five different mixes were cured and complete physical data were obtained. These data are so voluminous that only a brief summary can be given. (Tables I11 and IV) PURE-GUMMIX, No ACCELERATOR-Table 111 presents the summarized data obtained in a pure-gum mix. All the different types of rubber are shown to increase in rate of sulfur combination after heating. This checks the hand observation of time of cure based largely on tear, which is given in columns 2 and 3. In spite of this fact the modulus a t 800 per cent and the stiffness index have decreased except in the case of roll brown crepe, even a t the same time of cure. Examination of the tensile and elongation figures shows that the last part of the stress-strain curve is as high for the heated sample as for the original. This change in the form of the stress-strain curve is discussed later. It should be noted in this table, as well as in most of those following, that roll brown crepes show different physical properties than the other types of rubber investigated. If the stress-strain curve is plotted, that of roll brown crepe will be found to be much steeper than any of the others. Thus the stiffness index (difference between modulus a t 600 and 800 per cent elongation) of roll brown is usually increased considerably by the heat treatment. Other rubbers may not show this increase in stiffness index, because the curve is flatter at the 600 to 800 per cent elongation, but may have tensiles a t break equal or superior t o those of roll brown crepe. The best cures for sprayed latex were not obtained, the 1 hour and 30 minute cure being overvulcanized. In the case of the water-extracted sample both the stiffness index and modulus are lowered by heating, while in the unextracted sample they are increased. This may be due to the fact that the rate of cure was but little increased in the extracted sample and enormously increased in the unextracted. The combined-sulfur figures are evidence of the truth of this statement. It is, of course, obvious that a water-soluble material has been removed, which on hydrolysis is a strong accelerator of vulcanization. MERCAPTOBENZOTHIAZOLE ADDEDAS ACCELERATOR (Table IV) -Formula 1. This formula is the one used by Dinsmore and Zimmerman,' which cures an average crepe or sheet rubber in 1 hour a t 125" C. (20 pounds or 1.4 kg. per sq. cm. steam). Formula 2. A t this time and with this accelerator it occurred to the writers to study the effect of time of heating and the effect of dry heat as compared with moist heat. Using Formula 2, three samples of smoked sheets, all taken from the same piece of rubber, were heated as stated. It is evident that the cure effect Table 11-Effect RUBBER
Pale crepe T Roll brown S A Smoked sheet V V Acetone-extracted smoked sheet V V Smoked sheet S S Sprayed latex C Sprayed latex C , HzO extracted Evaporated latex
3.09 1.60 1.60 0.71 3.13 3.46 2.37 3.56
3.86 2.72 1.96 1.88 4.28 5.82 4.29 7.65
On summing up the effect of heating upon the cure with various accelerators, there appear to be two separate and entirely independent influences at work. The first of these factors seems t o be strictly chemical in its nature and its effect is noted by: (1) increase in acetone extract and change in nitrogen distribukion, as shown in Table 11; ( 2 ) acceleration of cure, especially in the case of mercaptobenzothiazole; (3) failure of acetone to remove the body which undergoes change on treating; and (4) removal by water of a portion
of Heat on Various TvDes of Rubber Na
h-2 I N RESIDUE
231 109 236
300 163 311
0.05 0.08 0.168
0.41 0.47 0.47
305 411 333
0.24 0.13 0.19 0.12
0.34 0.31 0.29 0.23 0.40 0.38 0.50 0.26
253 381 265
0.16 0.15 0.292 0.13 0.38 0.20 0.39 0.33
353 665 502
285 345 282
plasticity figures and in the form of the stress-strain curve. In this case also, the rate of cure and sulfur combination is increased; the rate of physical cure is also increased as judged by hand d s t s with emphasis on tear. The general position of the stress-strain curves is changed toward the load axis by heating, except in the case of sprayed latex. The combined-sulfur figures show that heating has little, if any, effect upon the rate of cure of sprayed latex, while the lowering of the modulus and IND. ENQ.CHEM.,17, 144 (1926).
stiffness index is peculiar to this type of rubber. It seems probable that the high stiffness index Of the roll brown rubbers as well as the sprayed latex may be explained as in the discussion of Table 111 and in a later section of this paper. The low stiffness index of pale crepe T might be open to question but for the fact that the time-stiffness curve at 700 per cent is almost flat a t this point, increasing only 4 in 30 minutes additional cure. HEXAMETHYLENETETRAMINE ADDEDAS ACCELERATOR-The most noticeable feature of these data is the definite lowering of physical properties in smoked sheets after heating and the accompanying movement of the stress-strain curves toward the axis of elongation. The same effect is true in a lesser extent of roll brown crepe, but barely noticeable in pale crepe. DIPHENYLGUANIDINE ADDED AS ACCELERATOR-The effect of heating was definitely to lower the quality of the diphenylguanidine stocks in every case. The samples also had a decidedly poorer tear than the originals, as well as lower tensile and modulus. The rate of cure, judged by hand tests and combined sulfur, was unaffected. ETHYLIDINE ADDED A S ACCELERATOR-The effect on these stocks is similar to the effect on diphenylguanidine stocks The rate of cure as judged by hand tests and combined sulfur was not increased. The stress-strain curves approach the strain axis and the physical properties are lower in all cases except that of roll brown crepe D D, which could not be repeated owing to loss of the sample.
increases with time of heating. In the case of the sample heated dry in a mold, the cure effect is present although weak. In this sample, as in those heated wet, the effect of heat shows up in the
0.58 0.56 0.75 0.56
of the material which undergoes change. The second factor seems to be physical and is possibly due to an altered structural condition. It is perhaps closely connected with the greater plasticity of the uncured rubber. The effect on the cured rubber may be summed up as follows: (1) There is a tendency to produce a softer stock with a somewhat different form of stress-strain curve. (2) The explanation of the low results with diphenylguanidine and ethylidene aniline is not to be found in the poorer innate qualities of the rubber, for the same heated samples produced
INDUSTRIAL AND ENGINEERING CHEMISTRY satisfactory results in other mixes. The phenomenonmay be due to the specific action of certain substances. Extra amounts of stearic acid in the presence of ZnO do not increase the rate of sulfur combination, but do greatly improve certain physical properties. Additional free fatty acids are probably formed by heating, as noted in Table 11. (3) The cure effect is present t o a greater extent in the presence of an excess of moisture over that found in the rubber, pointing to hydrolytic action. Effect of Heating upon the Stress-Strain Curve
. . L
P m a
As was stated in the discussion of Table 111, a difference in the form of the s t r e s s - s t r a i n curve was noted on all heated rubbers. Regardless of whether the general change in position of the curves has been toward or away from the strain axis (whether the modulus and tensile have been lowered or raised by heating), if a single curve of each stock can be found in the same general position on a stressstrain chart, the one made from the heated rubber will have a greater convexity toward the strain axis. In other words, that portion of the curve below 800 per cent elongation in pure gum and below 600 per cent in accelerated stocks is flatter after heating than in unheated rubber. At lower e l o n g a t i o n or just before break the heated rubber may have a slightly higher modulus than the unheated; but during the middle part the arc of the curve swings farther to the right. This is noticeable in nearly all the curves, and is shown in Figure 1. Sometimes the difference is striking. In other cases it would not be noticed upon casual inspection, but in 90 per cent of a very large number of comparisons it was possible to pick the heated rubber from the shape of the stress-strain curve. It is interesting to note that the difference in shape persists after 9 days' aging in the Geer oven, 16 hours in the Bierer-Davis oxygen bomb,
Vol. 20, No. 5
h'ole-As was stated in the discussion of Table III, a difference in the form of the stress-strain curve was noted between roll brown crepe snd the other types of rubber investigated. A typical cure for brown crepe seems to be a shorter stress-strain curve giving a much steeper slope at the proper tensile. If brown crepe is cured to give the same slope as pale crepe or smoked sheet rubber it is undercured and flabby.
A sample of smoked sheet heated dry showed the same type of curve. Whether this type of curve is more or less desirable than the type which more nearly approaches Hooke's law is an open question. A rubber of this type deforms easily up to a certain point and suddenly becomes exceedingly stiff and very difficult to break. Whatever other changes may have taken place upon heating, it is obvious that the proteins were profoundly affected, Undoubtedly, hydration and hydrolysis took place to a large extent. It is fairly well known that rubbers having widely different degrees of protein hydration may be prepared from the same latex. Those containing highly hydrated protein are softer in texture than those of low hydration. This fact probably explains the greater plasticity of the rubber before milling and curing. It is possible that the hydrated rubber is less severely broken down during milling owing to the allowance by the protein of greater slippage between the structural units. I n this case the structure of the finished cured sheets of heated rubber would be more like the original structure than the unheated ones. It must be admitted that the suggested explanation is given upon a basis of very incomplete facts, but it is believed to be warranted in view of the current interest in the spheroidal theory. Differences of this kind in the type of the stress-strain curve are frequently met in the study of pigments. They have been noted by the authors in the case of both zinc oxides and carbon blacks. Effect of Heating upon Aging
Although the aging studies were fairly comprehensive, no attempt has been made to arrive at more than qualitative conclusions. Three age tests were run on each stock: (1) 9 days in Geer oven a t 70" C.; (2) 16 hours in Bierer-Davis oxygen bomb; (3) 1 year natural aging. In all cases heated rubbers were equal or superior to the unheated as judged by modulus, tensile, and elongation. A possible explanation of this is that heating causes the natural antioxidant to become more reactive, through some internal change in the rubber structure. One rather remarkable feature of the diphenylguanidine stocks was that in several cases the year-old samples of heated rubber were equal to the unheated aged samples, although they were much inferior when fresh. Cause of the Increase in Rate of Cure
A review of the literature shows that several investigators have noted changes in rate of cure due to various naturally occurring products. The data, while somewhat conflicting, are presented. Frank* claimed most amino acids to be without effect in rubber-sulfur mixes. Garters found that one amino acid, leucine, shortened the time of cure of a pure-gum mix from 115 minutes to 105 minutes. Eatonlo investigated tyrosine, which proved to be without effect. Stevensll added peptone and casein to nearly nitrogen-free rubber and obtained almost as fast a cure as in the original rubber. Eaton'* and also Eaton and Grantham13 added peptone and casein to rubber-sulfur mixes without causing Rubber I n d . , 1914, 144. Arch. Rubbercultuur, 1, 377 (1917). 10 M Q ~ Q YAgr. Q ~ J , 6,319 (1918). 1 1 Kolloid-Z., 14,91 (1914). 1% MQtayQnAgr. J . , 6, 84 (1918). 18 J . SOC.Chrm. Ind., 56, 722 (1916). 8
INDUSTRIAL A N D ENGINEERING CHEMISTRY
W 40 W
,08"Go" 3--IPO a008 ;b
00000000 I O+I I I I e
o c n
.N .W r-
0 o c
W R c1
?Es C Pcn W
P N N W
.N N W
NN N I O
: 2 ?
35 3 i z
-NNNNNN W O r N U l O N
mmmm*mm O N O P W P W ooogoCAo
INDUSTRIAL A N D ENGINEERING CHEMISTRY
482 CLASS Amino acids: Monoaminomonocarboxylic Monoaminodicarboxylic acid Amino acid containing phenyl group &!fur containing amino acid Nitrogeneous bases: Heterocyclic
Table V-Action MATERIAL Alanine, glycine Aspartic acid Tyrosine Cystine
Quinoline Creatine Aliphatic Tri-n-propylamine Putrefactive bases: tetramethylenediamineo (putrescine) Proteins: hydrolysis products Hydrolyzed glue Peptone
Vol. 20, No. 5
of Protein Products on R a t e of Cure PUREGum
N o action No action N o action No action
Marked stiffening action No action No action N o action
h-o action No action No action
Stiffens but does not accelerate Vulcone, same as mercapto Stiffens but does not accelerate Vulcone, same as mercapto Slight activation
Accelerates and stiffens Accelerates and stiffens
Activates and stiffens Activates and stiffens
A c e r a t e s and stiffens
Glucosides Tannin Enzymes a A stiffer stock is obtained in 5 minutes report by W. W. Vogt).
Sicohin Retarder in all cases Non-glucosidal tannin No action Activates Fleischman’s yeast No action Activates at 141’ C. with 1 per cent of this materia! than is obtained in 150 minutes at 141” C. without it (unpublished
Activates and stiffens all accelerated stocks tried Activates and stiffens hexa, D. P. G..no action in Vulcone
SliRht retarder ...... -..
any acceleration. Recently Eaton and Bishop14 found that, extracted rubber was used since the action of the acetoneof several alkaloids tried, only one, emetine, had any marked soluble constituent^^^ was known and would therefore not accelerating value in a rubber-sulfur mix. hinder the study. The thinly milled smoked-sheet rubber, I n the writers’ study of the causes of increased rate of cure, after acetone extraction, was heated in the autoclave with they have attacked the problem from two standpoints: (1) water as described under the section “Effect on Chemical the compounding of some of the known protein decomposi- Characteristics.” The rubber was then sheeted out on a tion products and such other substances as were thought corrugated mill (“cracker”) and the water extract thus might be present in rubber; (2) a study of the water-extract- obtained was united with the water taken from the autoclave. able matter obtained after heating. The number of plant The sheeted-out rubber was rolled up in cloth which had been products which might be present in cured rubber is rather previously boiled out in water. The rubber was then soaked appalling and includes alkaloids, amino acids, enzymitic in water a t 80-90” C. until fresh water added daily did not products, carbohydrates such as sugar or starch, putrefaction become colored in 24 hours. Fifty pounds (23 kg.) of rubber bases, gums, waxes and resins, saponin, tannin, proteins were extracted in this way using about 50 liters of water, with their intermediate and final decomposition products which was acidified to prevent loss of volatile bases and and other nitrogenous bases. concentrated on the steam table to a volume of about 1.5 The writers were particularly interested in nitrogenous liters. To this were added the water taken from the autobodies, as the odor of the rubber on removal from the auto- clave and that removed from the hydrolyzed rubber while clave, as well as the nitrogen determinations as listed in sheeting out. On cooling this concentrated solution a brown, slimy preTable 11, indicated a profound change in the nature of the cipitate settled out, which was not again soluble in water nitrogen-containing bodies. ADDITIONOF KNOWN PROTEIN DECOMPOSITION PRODUCTS-but was easily soluble in alcohol. This material resisted all As a f i s t step in determining what materials influenced the attempts to purify it and remained a brown, molasses-like rate of cure or physical properties, several representative product, practically odorless. The water solution was then further concentrated to a members of the different classes were compounded, cured, and tested. These materials were tested in a 100 rubber-10 volume of about 500 cc. per 50 pounds (23 kg.) of rubber. sulfur mix using 0.5 to 1.0 per cent of substance being studied. No further crystallization took place on cooling, but by apAnother series consisted of 100 rubber, 6 ZnO, 2.75 sulfur, plying first a chloroform extraction and then the butyl 0.5 mercaptobenzothiazole, and 0.10 to 0.25 per cent of the alcohol extraction method of Dabin18 the solution was divided natural product. The second formula was used because this into three parts: (1) chloroform-soluble, water-soluble; (2) accelerator is somewhat more sensitive to added materials butyl alcohol-soluble, chloroform-insoluble, water-soluble; than other commercial accelerators. Some of the materials (3) butyl alcohol- and chloroform-insoluble and water-soluble. were also tested in storks containing other accelerators, such A better understanding of this procedure may be obtained as Vulcone, diphenylguanidine, etc. The results of these from Table VI, The apparatus used for the butyl alcohol extraction was of the Kut~cher-Steudell~ type and provides tests are given in Table V. The principal fact to be noted is that the best activators a method for the hot extraction of one liquid by another by of accelerated stocks are the least complex molecules-e. g., constantly bringing fresh solvent into contact with the liquid glytine-while the best accelerators of the pure-gum mix being extracted. I n these three solutions there may be are those in which there is a strong base, not impeded by an present ayino acids or other protein decomposition products, acid radical. (The hydrolyzed glue contained free amines.) alkaloids, or other nitrogen bases, glucosides, carbohydrates, The action of peptone is peculiar; it contained no free amines sugars, gums, and tannin. Water solutions of the above and simple amino acids, for it would then have activated three fractions were prepared and tested by a large number the mercaptobenzothiazole cure, yet it apparently shares of reagents for the above-mentioned substances. The followsome property of hydrolyzed glue, to cause it to react in the ing results were obtained: same manner in a rubber-sulfur mix. 1-No part of the hydrolysate contains any material that will ISOLATION OF HYDROLYS~S PRODUCT OF NATURAL reduce Fehling’s solution, such as sugars, starch, and certain ACCELERATOR-Since such differences in rate of cure were glucosides. Negative tests were obtained for tannin by several those which would distinguish it from noticed before and after heating rubber, it was believed that reagents, particularly No free amines were found. either the natural accelerator or a clue to its identity obtained saponin. 16 Whitby, J . Chem. SOC.(London), 1926, 1448; also Rubber Age (Lonby isolating its hydrolysis product might be isolated from a 401 (1926). water or alcohol extract of the heated rubber. Acetone- don),166,Biochem. J., 12, 980 (1918). 24
Malayan Agl. J.. 14, 8 (1926).
J . Chem. SOC.(London), 84, SOA (1904).
INDUSTRIAL AND ENGINEERING CHEMISTRY
2-Positive tests were obtained for saponin, proteins, and other carbohydrates and their hydrolysis products .with the Molisch test and others. Positive tests were also obtained for alkaloids and other nitrogen bases. Solution of Hydrolysate Concentrate to 1500 cc. per 23 kg. rubber
Table VI-Water Ppi. I
Concentrate to 500 cc. and shake *th CHClt
CHClr jnsoluble Boil wi$h BuOH BuOH ihsoluble Ppt. I1
BuOH sodble I
Non-ciystalline solid obtained by distilling off BuOH under reduced pressure Ppt. IV
As will be noted, the addition of these substances activated mercapto and produced both a stiffer stock and a faster cure. Fractions from Wuter Extract. Other samples prepared from a similar hydrolyzed rubber gave even more striking results. Ppt. IV-a, butyl alcohol-soluble, non-crystalline residue. This sample was 7 months old when compounded and had a disagreeable, putrid odor. Ppt. IV-b, same age and preparation as IV-a, but had no odor whatever. Ppt. IV-c, same as IV-a, but freshly prepared. Ppt. 114,butyl alcohol-insoluble, water-soluble, non-crystalline residue.
Crystals Ppt. I11
The resinous nature of the different fractions may be due to certain natural resins, waxes, and gums which are not soluble in acetone but are soaked out by water after hydrolysis. It now remained to separate and identify these products, if possible. No one fraction amounted to more than 0.1 per cent of the rubber, the greater part of the water extract being inactive, resinous material. Alcohol as Extractiv Medium. It was thought that the use of alcohol as an extracting medium might give separations which could be more easily purified than those from water. Therefore, a fresh lot of smoked sheets, about 25 pounds (11 kg.), was acetone-extracted, hydrolyzed, and then extracted with alcohol in a large metal extractor. On concentration the alcohol extract yielded a small quantity of flat, brownish crystals which could not be purified, as the water extract had yielded a similar, though slimy, precipitate. These crystals were numbered Ppt. I. The filtrate was next taken to dryness, no further crystallization having taken place, taken up in water in which the gummy residue was entirely soluble, and then extracted hot with butyl alcohol until fresh additions of the butyl alcohol were colorless. The chloroform extraction was omitted in this case and three products were obtained.
Three per cent of these materials were used to activate mercapto stocks with the results shown in Table VIII. Table VIII-Effect
of Adding Water Extract8 to Mercapto Stocks BESTCURB STIFFNESS (125’ C.) INDBX TENSILE
MATERIAL ADDED Control Ppt. IV-a Ppt. IV-b Ppt. IV-c Ppt. 11-b
Minutes 100 45 100 45 100
54 101 69 92 58
Kg./rq. cm. 132 200 159 180 152
I n this case we have to deal with putrefaction bases, present in IV-a, which undoubtedly have considerable accelerating and stiffening action. The increase due to the action of putrefaction bases is represented by the difference between IV-a and IV-c. The latter is the same as IV in Table VI1 and activates similarly, considering the amount used. 114 is similar to I1 in Table VII. The noteworthy fact about these materials is that, while they have the ability to activate mercaptobenzothiazoleaccelerated stocks, they are practically without effect in a pure-gum mix. If this is true, then none of them is the natural accelerator, and none the cause of variability between different lots of the same type of rubber. This is further indicated by Tables I11 and IV, which show that the effect of heat is not to remove variability but to increase it. It is possible however to correlate the effect of these extracted substances with that of the pure compounds tested Ppt. IV, butyl alcohol-soluble, non-crystalline material, which, in Table V. If we suppose that hydrolysis has been comaccording t o the scheme of Dakin contains such amino acids plete and the hydrolysate contains only the final splitting as proline and other heterocyclic compounds. The writers have products, we find that these are the materials which do not shown that quinoline, another heterocyclic compound, has a slight accelerate alone, but do have the ability to activate accelerastiffening action on mercapto-accelerated stocks, much in the same order as this crude material. From this fraction Ppt. IV tors-viz., the simplest amino acids and nitrogenous bases. The intermediate splitting products and more complex a white crystalline solid was obtained, which after repeated crystallizations from alcohol melted sharply a t 205” C. The nitrogenous materials have a slight accelerating action in melting point of proline is 208’ C. However, this substance pure-gum mixes. analyzed to a CCcompound, whereas proline is a Ca, and the In summing up the chemical causes of the increased rate writers were not able to identify it. The analysis was as follows: of cure, we may say that (1) amino acids, except the simplest carbon, 44.72-45.30; hydrogen, 6.72-6.84; nitrogen, 12.03 per cent. Such a compound would have a formula of CaHsOzN. ones, are without effect in pure-gum cures; (2) amines and There was not enough sample for a molecular weight determi- nitrogen bases activate accelerated stocks, particularly mernation. Ppt. 111, butyl alcohol-soluble, separates out as minute captobenzothiazole; (3) alkaloids exert some accelerating crystals on cooling. In the Dakin scheme these crystals are and activating influence. The writers believe that all three monoamino acids, and since they seemed very uniform under the types of compounds are present in rubber, their presence microscope there were probably no other substances present. having been indicated in the water extract of heated rubber, They melted at 164” C. and that they are the chemical cause of the peculiarities of Ppt. 11, butyl alcohol-insoluble, water-soluble, non-crystalline residue composed of diamino and dicarboxylic acids and a mix- heated rubber. ture of other plant substances.
When these materials were added to a mercapto stock in the proportion of 2 per cent on the rubber, the results shown in Table VI1 were obtained. of Adding Alcohol Extracts to Mercapto Stock BESTCURE S T ~ ~ N E S S MATERIAL ADDED (125’ C.) INDEX TENSILE Minnlcs Kg./sq. rm. Control 45 48 124 Ppt. I 30 57 117 Ppt. IV 30 69 144 Ppt. I11 -45 45 136 Ppt. I1 45 64 136
Thermal Expansion of “Stainless Iron” Alloys The Bureau of Standards has recently completed a n investigation on the thermal expansion of low-carbon iron-chromium alloys of the “stainless iron” type. These alloys are being used to a n increasing extent for various purposes, such as parts of steam turbines, devices for handling acids, and in the manufacture of other articles that must resist corrosion. Results on their expansion for various temperature ranges between room temperature and 1000” C. have now been published in Scientific Paper 570. This material expands about 17 per cent less than pure iron for the range from room temperature to 1000” C.